and decay times, a poorer solvent has to be used in which the coils are smaller. Toluene as the theta solvent at 37 "(214 was chosen for such a study despite the poorer optical quality of glasses formed a t 77 K. The results, which will be published elsewhere, show that the general spectroscopic behavior is rather similar in both solvents. Intramolecular triplet-triplet annihilation is therefore likely to be the cause of delayed fluorescence of PVCA in these solvents. The process is favored by the slow first-order triplet decay in carbazole derivatives. In M solutions in MTHF at 77 K we measured ~p = 8.2 s (PVCA VI) and T P = 7.8 s (N-isopropylcarbazole). Neglecting secondorder decay, we roughly estimate that on the average we have one triplet/macromolecule if the molecular weight is 2 x lo4. At higher molecular weights the chance to meet two or more triplets together a t the same molecule increases and delayed fluorescence can occur (Figure 4), competing with phosphorescence. Delayed fluorescence decays much faster than phosphorescence ( TDF = 3-4 ms in toluene), which indicates that the triplets whose decay is observed in phosphorescence are not the mobile triplets causing delayed fluorescence. Similar conclusions have been drawn by Yokoyama et a1.16 in a recent study of the phosphorescence of PVCA in which strong evidence from quenching experiments is presented for a trap (probably carbazole end groups) as origin of the phosphorescence. Recently, delayed fluorescence due to photoionization and recombination has been observed in carbazole/ether at 77 K.15 Using the monomeric model N-isopropylcarbazole in MTHF
we did not detect any delayed fluorescence. In the case of the polymer, the molecular weight dependence seems to exclude photoionization as a major cause of delayed fluorescence. A final decision about the mechanism, however, can only be made after a kinetic analysis of the quantitative study now under way.
Acknowledgment. This work has been performed as part of the Battelle Institute program in physical sciences.
References and Notes Paper presented in part a t the 3rd European Symposium on Polymer Spectroscopy in Uxbridge, London, April 1974. (a) R. F. Cozzens and R. B. Fox, J . Chem. Phys., 50,1532 (1969); (b) C. HBlSne and J. W. Longworth, ibid.,57,389 (1972). W. Klopffer and D. Fischer, J . Polym. Sei., Polym. Symp., No. 40, 43 (1973). M. Yokoyarna, T. Nakamo, T. Tamamura, and M. Mikawa, Chem. Lett., 509 (1973). A. C. Somersall and J. E. Guillet, Macromolecules, 6,218 (1973). G. E. Johnson, J . Chem. Phys., 62,4697 (1975). M. Bazin, R. Santus, and C. HBlSne, Chem. Phys., 2,119 (1973). P. Avakian, R. P. Groff, A. Suna, and H. N. Cripps, Chem. Phys. Lett., 32, 466 (1975). W. Klopffer and H. Bauser, 2. Phys. Chem. (Frankfurt am M a i n ) , 100, 25 (1976). R. D. Burkhart, Macromolecules, 9,234 (1976). D. Fischer, J. Appl. Phys., 44,1977 (1973). W. K1ooffer.J. Chem. Phvs.. 50. 2337 11969). (13) G. Sitaiarnaiah and D. Jacobs, Polymer, 11,165 (1970). (14) N. Kuwahara, S. Higashida, M. Nakata, and M. Kaneko, J . Polym. Sci., Part A-2, 7,285 (1969). (15) D. Muller, M. Ewald, and G. Durocher, Can. J . Chem., 52,3707 (1974). (16) M. Yokoyama, T. Tamamura, T. Nakano, and H. Mikawa, J . Chem. Phys., 65,272 (1976).
Temperature Dependence of Hydrogen Bonding in Toluene Diisocyanate Based Polyurethanes C. S. Paik Sung* la and N. S. Schneiderlb Department of Materials Science and Engineering, Massachusetts Institute of Technology, Cambridge, Massachusetts 02139, and Polymer and Chemistry Division, Army Materials and Mechanics Research Center, Watertown, Massachusetts 021 72. Received October 7,1976
ABSTRACT: The temperature dependence of hydrogen bonding in 2,4-TDI and 2,6-TDI based polyurethanes was investigated using simple procedures to resolve hydrogen bonded and nonbonded NH and carbonyl. The fraction of hydrogen bonded carbonyl was used as a measure of the extent of interurethane hydrogen bonding. The onset temperature for dissociation of both hydrogen bonded NH and carbonyl in 2,6-TDI polymers occurs at 65 "C, independent of urethane content and well below the melting temperature of crystalline hard segment structure (130 to 170 "C). For 2,4-TDI polyurethanes the onset temperature for dissociation of hydrogen bonded NH occurs a t 40 to 60 "C, close to the transition temperature for amorphous domain structure, but there is little change in hydrogen bonded carbonyl up to the highest temperature studied (150 "C). Heats of dissociation were about 4 kcal/mol in both series. The 2,4-TDI results demonstrate the preferential dissociation of urethane to soft segment bonding and, by contrast with the lower stability of interurethane bonding in 2,6-TDI samples, suggest that hydrogen bonding to the 4 position of the TDI ring is stronger than the 2 position. The structural implications of the 2,6-TDI and 2,4-TDI results are discussed. Overall, the behavior indicates that the cause of hydrogen bond dissociation bears little relation to the state of structural organization.
In previous work, two series of segmented polyurethanes, one based on 2,4-toluene diisocyanate (TDI), the second on 2,6-TDI, were investigated to determine the effect of asymmetric placement of the isocyanate groups on domain structure, microphase segregation, and polyurethane properties.2a Quantitative infrared analysis of the urethane NH and carbonyl bands was carried out as a means of assessing the degree of phase segregation,2bunder the assumption that the fraction of NH involved in interurethane bonding was a direct measure of phase segregation. The infrared results showed that ex-
tensive mixing of hard and soft segment occurred in the 2,4-TDI polymers and provided a basis for explaining the rapid increase in the soft segment T , which occurs with increasing urethane content in these samples. In the present work, we have attempted to examine the relation between hydrogen bonding and the higher thermal transitions. The first such studies were carried out by Seymour and Cooper3 to determine the relation between hydrogen bonding and domain morphology in MDI based polyurethanes. They showed that the transitions observed by DSC
H Bonding in Toluene Diisocyanate Based Polyurethanes
Vol. 10,No. 2, March-April 1977
Chart I soft segment
hard s e g m e n t
could be moved to higher temperatures whereas the onset temperature for hydrogen bonding dissociation, obtained from infrared analysis of the NH absorbance, remained unchanged a t 70 to 80 "C. These results lead to the conclusion that hydrogen bonding, in fact, played only a secondary role in the structure and properties of the hard segment domains. In the 2,4-TDJ based polyurethanes only weak domain related transitions below 100 "C are observed, due to the amorphous nature of the domain structure, and these transitions are insensitive to annealing. In the 2,6-TDI samples the domain structure is crystalline. Therefore it is of interest to determine whether the relation between hydrogen bonding and domain transitions for these samples is consistent with that observed by Seymour and Cooper. Since the urethane groups are distributed between the domain structure and the soft segment phase, we looked a t the behavior of both NH and carbonyl groups as a function of temperature using simple procedures for resolving hydrogen bonded and nonbonded components of the two absorption bands. The changes in the carbonyl band monitor the interurethane hydrogen bonding and, therefore, the process occurring mainly in hard segment domains. Despite difficulties in the data analysis, the results lead to conclusions which in part are consistent with Seymour and Cooper's work but also represent behavior and problems not previously observed.
2,6-TDI Based Polyurethanes. In our previous publication,2a we reported that segmented polyurethanes based on symmetric 2,6-toluene diisocyanate were semicrystalline and opaque. IR analysis on these polymers showed that 80% of NH groups are bonded to carbonyl groups in the urethane linkage. This implies that almost all the urethane segments reside in hard segment domains, while the remaining 20% of NH groups are bonded either to soft segment ether groups or to urethane alkoxy1 groupszb Figure 1 shows the effect of temperature on the NH region of IR spectra for a representative 2,6-TDI polyurethane, 2,6-TDI-3. At 0 "C, all the 2,6-TDI polymers exhibit NH absorption bands, which are almost completely hydrogen bonded, centered at 3300 cm-l. As the temperature is raised, the hydrogen bonded NH absorption decreases while a free NH absorption shoulder develops which is centered a t 3460 cm-'. Since the extinction coefficient of free NH groups is about one third of that for hydrogen bonded NH groups: the increase in free NH absorption is not as great as the decrease in bonded NH absorption. At 0 "C, curve resolving using the Du Pont 310 curve resolver indicated that 95-97% of NH are
Wavenumber, ( c m " )
Experimental Section Polymers. The polymers investigated in this study were the two series of polyether polyurethanes, one based on 2,4-TDI and the other series based on 2,6-TDI as shown in Chart I. The soft segment is poly(tetramethy1ene oxide) of molecular weight 1000. The detailed synthesis of these polymers was described previously.2aThe molar ratio of TD1:butanediol:polyether was varied in five equal steps from 2:l:l to 6:5:1. In sample designation, the number of moles of diisocyanate per mole of polyether is indicated by the integer which follows the specified TDI isomer. Infrared Temperature Studies. A Beckman-12 infrared spectrophotometer was used with a variable temperature unit (Wilks Model No. 19) connected to the temperature controller (Wilks Model No. 37). Subambient temperature was obtained by passing a stream of liquid nitrogen through in. copper tubing soldered to a copper plate which was attached to the salt plate holder. The temperature range was from -20 t o 160 "C and the temperature was controlled within fl "C. The chamber containing the cell was flushed with dry nitrogen to avoid the condensation of moisture on the salt plate. All the samples were prepared by casting from DMF solution (-2% by weight) and drying in a vacuum oven until there was no evidence of residual solvent. Small-Angle X-Ray Scattering. A Kratky camera was used t o obtain the angular dependence of scattered intensity for 2,4-TDI polyurethanes. Radiation was supplied by a graphite monochromated Noretco copper fine-focus tube operated a t 50 kV and 30 mA. The Kratky camera was equipped with automatic step scanning, counting, and printing devices.
Figure 1. Temperature dependence of the NH region in the IR spectrum for 2,6-TDI-3.
Temperature T *C
Figure 2. Estimation of fraction of bonded NH in 2,6-TDIpolyurethanes (fraction of bonded NH = ( A T / A ~X) 0.95).
Figure 4. Gibbs-Helmholtz plot of In k vs. 1/T for the dissociation of bonded NH groups for 2,6-TDI-5.
, , , , , , ,J 40
Figure 3. Fraction of bonded NH groups and carbonyl in 2,6-TDI polymers as a function of temperature.
hydrogen bonded. The fraction of bonded NH a t higher temperatures was then calculated by comparing one-half of the total bonded area, as shown in Figure 2, with that of the reference spectra at 0 "C. Figure 3 illustrates the results of this analysis as a function of temperature for the various 2,6-TDI polymers. The onset of the dissociation of hydrogen bonded NH groups appears to occur around 60 to 70 "C for all of 2,6-TDI based polyurethanes. The dissociation of hydrogen bonded NH groups for these polymers follows an equilibrium process governed by the following equation above the onset temperature;
d In k/d( UT) = - AHIR where k , the equilibrium dissociation constant, is equal to [cf]'/[ch]with Cf the fraction of free NH and c h the fraction of bonded NH. Figure 4 shows a typical plot of In k vs. 1/T, whose slope gives AH/R, where AH is the dissociation energy of hydrogen bonded NH groups. It should be noted that when plotted in this form the data show a clearly defined transition in behavior for the values above 1/T = 3.0 X despite the scatter. Some care must be exercised in interpreting the discontinuity in NH absorbance or in the fraction of bonded NH as an indication of a transition. For certain values of the heat and entropy of dissociation, an apparent transition will occur in the absorbance or fraction of bonded NH even when equilibrium behavior is followed over the temperature range of interest (see Appendix). The results from the analysis of the data in Figure 3 are summarized in Table I, where it can be seen that AH values of 4-5 kcallmol of hydrogen bond are obtained. The values seem to be independent of urethane concentration and are reasonable for the dissociation of hydrogen bonded NH group^.^ The small variation in AH values within the 2,6-TDI polymer series, in part, reflects the error in estimating the initial bonded fraction at 0 "C. For example, a 5% decrease in
Figure 5. Temperature dependence of the carbonyl region in the IR spectrum for 2,6-TDI-3.
Table I The Onset Temperature and AH of Dissociation of Hydrogen Bonded NH Groups in 2,6-TDI Polyurethanes
Polymer 2,6-TDI -3 -4 -5 -6
Onset temp, "C
AHlmol of hydrogen bond, kcal
66 60 72
the bonded fraction at the reference temperature would lower AH values by as much as 1 kcal/mol of hydrogen bond. Since 80% of NH groups in 2,6-TDI polyurethanes are bonded to urethane carbonyl, the dissociation of NH groups must reflect a process occurring almost exclusively within the hard segment domain. However, it is complicated with a small contribution from dissociation of NH groups bonded to soft segment ether which cannot be distinguished on the basis of the results of Figure 3. Therefore, we investigated the temperature dependence of hydrogen bonded carbonyl groups to obtain information which is more sensitive to the changes in the hard segment domains. The behavior of the carbonyl absorption is illustrated in Figure 5 for a representative 2,6-TDI polymer, 2,6-TDI-3. As the temperature is raised, hydrogen bonded carbonyl absorption at 1700 cm-' decreases and free carbonyl absorption at 1740 cm-l increases. In several samples it was apparent that both bonded and nonbonded regions of the carbonyl band consisted of a number of severely overlapping peaks. The fraction of bonded carbonyl was calculated based on peak height at 1700 cm-' for bonded carbonyl and at 1740 cm-1 for free carbonyl rather than peak area because of the difficulty of resolving these closely overlapping peaks and the results are plotted in Figure 3. Since the bonded peak
H Bonding in Toluene Diisocyanate Based Polyurethanes
Vol. 10, No. 2, March-April 1977 Table I1 The Onset Temperature and AH of Dissociation of Hydrogen Bonded Carbonyl Groups in 2,6-TDI Polyurethanes
m / m o l of hydrogen bond, kcal
60 60 68
3 3 4
Onset temp, Polymer
is broader than the nonbonded carbonyl, this will tend to overestimate the fraction of free carbonyl groups. As in earlier calculations, it was assumed that the extinction coefficients for free and bonded carbonyl are equal. The onset temperature for the dissociation of the bonded carbonyl is between 60 and 65 "C which is in the same temperature range for the analogous process involving NH groups. The dissociation energy, A H , was calculated for 2,6-TDI polymers by assuming 80% bonded carbonyl a t 0 "C, which was obtained by curve resolving. As summarized in Table 11, AH values of 3-4 kcal/mol are obtained for the dissociation energy of carbonyl groups. The values are somewhat smaller than those obtained from analysis of the NH band but again are independent of urethane concentration. The smaller values of 1H for the dissociation of carbonyl groups might be due to underestimation of the initial 0 "C value for bonded carbonyl or to discrepancies in the estimation of free carbonyl based on the relative peak height changes. These results support the conclusion that dissociation of hydrogen bonds in the 2,6-TDI samples occurs mainly in hard segment domains above the onset temperature. Some insight concerning the behavior of the urethane to ether hydrogen bonding can be gained from a comparison of the results for bonded NH and for bonded carbonyl in Figure 3 when plotted together as a function of temperature. It then becomes apparent that the two sets of data are nearly parallel and separated by a constant interval below the onset temperature for all three samples where the comparison can be made. Above the onset temperature, the behavior is somewhat variable. The results for the fraction of bonded NH and carbonyl continue on a parallel course in 2,6-TDI-4 but converge a t higher temperature in 2,6-TDI-5. The behavior below the onset temperature indicates that urethane bonding to proton acceptors other than carbonyl in all cases is stable up to the onset temperature. This may be contrasted with results on 2,4-TDI, to be discussed in the following section, where a decrease of about 10%in bonded NH occurs below the onset temperature without any change in the carbonyl distribution. If only urethane to ether bonding is considered, this would imply that such bonding is stronger in 2,6-TDI than in 2,4-TDI polyurethanes, a difference which is difficult to explain on the basis of the structure of the isomers. One possible way out of this dilemma is to invoke the contribution of urethane to alkoxy bonding which can occur within the highly ordered domain structure of 2,6-TDI polyurethanes. The persistence of this bonding in some degree well beyond the onset temperature indicates that it is comparable in strength to the urethane to carbonyl bonding. Urethane to alkoxy bonding would be present to only a minor extent in the 2,4-TDI samples since a large fraction of the urethane segments are distributed in the soft segment phase. This explanation implies that the infrared values for the fraction of nonbonded carbonyl overestimate the amount of urethane soft segment mixing. In fact, this conclusion is consistent with the observation that values for the soft segment glass transition
Figure 6. Temperature dependence of the NH region in the IR spectrum of 2,4-TDI-2.
calculated from the infrared results using the Fox copolymer equation are equal to or higher than the experimental values in the 2,6-TDI polyurethanes, but the calculated values fall well below the experimental values for 2,4-TDI samples.2b 2,4-TDI Based Polyurethanes. We reported that segmented polyurethanes based on asymmetric 2,4-toluene diisocyanate were transparent and amorphous and that their properties changed progressively from rubbery to plastic with increasing urethane concentration.2a IR analysis on these polymers revealed that 50% of NH groups are bonded to carbonyl presumably with the rest hydrogen bonded to the soft segment, thereby indicating extensive intermixing of hard and soft segment. Figure 6 shows the effect of temperature on the NH region of the IR spectrum for a representative 2,4-TDI polyurethane, 2,4-TDI-2. At 0 "C, NH groups show up to 95% hydrogen bonding with an absorption peak a t 3320 cm-l, while free NH groups (5%) exhibit a small shoulder a t 3460 cm-l. With increasing temperature, the hydrogen bonded peak decreases while the free NH peak develops. The fraction of bonded NH groups was obtained by the same procedure used for 2,6-TDI polymers. Figures 7a and 7b illustrate the results obtained as a function of temperature for all the 2,4-TDI polyurethanes. At higher temperatures, the method of taking a half of the bonded NH peak tends to overestimate the fraction of the bonded NH and the flattening of the curve in Figure 7b for 2,4-TDI-4 in the range of 80-140 "C may reflect this effect. In Figure 7, the discontinuity in the curves as drawn occurs a t about 40 "C for the first three samples and a t 60 to 70 "C for the two samples of highest urethane content. The values for all samples are summarized in Table I11 together with other pertinent data. In all cases the onset temperatures are well above the glass transition temperature of the soft segment phase and, in fact, fall in closer line with the Tz transition of hard segment domains (see Table 111) although the correlation is not exact. The dissociation energy AH is about 3-4 kcal/mol of hydrogen bonds for all 2,4-TDI polymers above the onset
456 Sung, Schneider
40 80 Temperalure, I T )
Figure 8. Temperature dependence of the carbonyl region in the IR spectrum for 2,4-TDI-2.